PRESENTED BYMr. Sudip M. MulikM.PHARM .I (PHARMACEUTICS) Under The Guidence of Prof. Mr. K. K. Mali FACULTY OF PHARMACY YSPM’S-YTC WADHE, SATARA.
INTRODUCTION PROPERTIES ANGLE OF REPOSE CARR’S INDEX COMPRESSION CYCLE FORCES INVOLVED IN COMPRESSION EQUATIONS CONCLUSION REFERENCES 2
COMPRESSION Reduction in bulk volume of material due to displacement of gaseous phase.CONSOLIDATION Increase in mechanical strength of material due to particle-particle interaction.COMPACTION It is the compression & consolidation of two phases (solid & gas) system due to applied force.
Itis defined as the reduction in volume of a powder owing to the application of a forces. Because of the increased proximity of particle surfaces accomplished during compression, bonds are formed between particles which provide coherence to the powder i.e. compact is formed.
Whenexternal mechanical forces applied to a powder mass there is reduction in bulk volume as follows o Repacking o Particles deformation • Elastic deformation-e.g. acetyl salicylic acid, MCC • Plastic deformation-at yield point of elastic. o Brittle fracture – e.g. sucrose o Micro quashing - irrespective of larger particles, smaller particles may deform plastically.
Compaction Consolidation It is defined as the It is increase in formation of solid mechanical strength of specimen of defined geometr y by powder material from particle- compression. particle interactions. The compression takes place in a die by the action of two punches, the lower and the upper by which compression force is applied.
Porosity (E)o Void volume Void volume = Bulk Vol – True Vol E = Void volume / Bulk Vol = V / VbThe relation bet compression & porosity is important because it determines rate of dissolution, disintegration & absorption.
Particle shape : Spherical smooth particles increases flow properties Density/Porosity : High density = Low porosity = Good flow Moisture High moisture = cohesion, adhesion = poor flow 10
Angle of Type ofrepose (in flowdegrees)Less than Excellent250 Angle of repose25-300 Good = tan-1(h/r)30-400 PassableMore than Very poor400 11
Carr’s consolidation Indexconsolidation Index = Tap density – Bulk density/Bulk density Carr’s Index Flow 5-15 Excellent 12-16 Good 18-21 Pair to passable 23-35 Poor 33-38 Very poor More than 40 Very poor Very poor 12
Process of compression Appropriate volume of granules in die cavity is compressed between upper & lower punch to consolidate material into single solid matrix which is finally ejected from die cavity as tablet. 13
Transitional repacking /Particle rearrangement Deformation at point of contact Fragmentation Bonding Decompression Ejection 14
During initial stage of compression particles are subjected to low pressure during this particles moves with respect to each other . Smaller particles enter voids bet larger particles as a result volume decreases & density increases. Spherical particles undergo lesser rearrangement than irregular particles. 15
Elastic : When force is applied deformation occurs & deformation disappears upon release of stress. Plastic : The deformation which does not completely recover after removal of stress. Yield strength : Force required to initiate plastic deformation
As compression force increases deformed par ticles star t undergoing fragmentation due to high load par ticles breaks in to smaller fragments leading to formation of new bonding areas . The fragments undergo densification with infiltration of small fragments in to voids. Some par ticles undergo structural break down called as brittle fracture. 17
Cold welding : When particles approach each other close enough (at the distance of 50µm) the unsatisfied forces present on their surface lead to formation of strong attractive forces/bonding Formation of strong attractive forces. This is called as cold welding. Fusion bonding : In the powder mass particles are in irregular in shape ,size & applied force to mass must pass through this bed of particles this transmission may lead to generation of heat .If this heat doesn’t disappear the raise in temperature could be sufficient to cause melting of contact points. This melt is cooled & solidifies that gives rise to fusion bonding.
The success & failure of intact tablet depends on stress induced by elastic rebound & the associated deformation produced during compression & ejection . As the upper punch is withdrawn from the die the tablet is confined in die cavity by radial pressure consequently any radial change during decompression must occur in axial direction. Thus capping is due to unaxial relaxation in die cavity at the point where punch pressure is released & some may occur at ejection. If decompression occurs in all directions simultaneously capping is reduced. 19
EJECTION As lower punch rises & push tablet upward there is continuous residual die wall pressure & energy may be expanded due to die wall friction . As the tablet is removed from die lateral pressure is relieved & tablet undergoes elastic recover y with increase (2- 10%) in the volume of that por tion of the tablet removed from the die. During ejection that por tion of the tablet within die is under strain so if exceeds the shear strength of the tablet, the tablet caps adjustment to the region in which the strain has been removed .
Various forces involved in the Compression Frictional force Distributional force Radial force Ejectional force
Frictional force Frictional forces are interparticulate friction & die wall friction. Interparticulate friction forces occur due to particle-particle contact & it is more significant at low applied load . These forces are reduced by using glidants e.g. colloidal silica . Die wall friction forces occur from material pressed against die wall & moved it is dominant at high applied load These forces are reduced using lubricants e.g. magnesium stearate.
Distribution Forces Most investigations of fundamentals of tableting have been carried out on single punch press or even isolated dies & punches with hydraulic press A force is applied on top of cylinder of powder mass consicder single isolated punch FA = Force applied to upper punch FL = Force transmitted to lower punch FD = Reaction at die wall due to friction at surface FA = FL + FD.
Compaction Force Because of difference between applied force at upper punch which affects material close to lower punch is called as Mean Compaction Force (FM). FM = FA + FL/2Radial ForceAs compressional force is increased any repacking of tableting is completed.
POISSON’S RATIO OF MATERIAL When force is applied on vertical direction which result in decrease in height (∆H) for unconfined solid body. The expansion is in horizontal direction (∆D). This ratio of two dimensional changes is known as Poisson’s ratio ( )גof material. גD = ∆D / ∆H The material is not free to expand in horizontal plane because it is confined in die at the same time a radial die wall force (FR) develops perpendicular to die wall surface. Higher Poissons ratio ( )גhigher FR value.
Ejection Force Radial die wall forces & die wall friction also affects ejection of the compressed tablet from the die. The force necessary to eject the finished tablet is known as ejection force. This force can eject tablet by breaking tablet/die wall adhesion. Variation also occurs in ejection force when lubrication is inadequate.
Heckel equation Heckel plot is density Vs applied pressure. Follows first order kinetics. As the porosity increases the compression force will increase. The Heckel equation is described as follows. It is based on the assumption that powder compression follows first-order kinetics, with the interparticulate pores as the reactant and the densification of the powder bed as the product. Where D= relative density of a powder P=compact at pressure P. Constant k = measure of the plasticity of a compressed material. Constant A =die filling and particle rearrangement before deformation and bonding of the discrete particles. Thus, a Heckel plot allows for the interpretation of the mechanism of bonding.
Kawakita equation The Kawakita equation is described as follows. This equation describes the relationship between the degree of volume reduction of the powder column and the applied pressure. The basis for the Kawakita equation for powder compression is that particles subjected to a compressive load in a confined space are viewed as a system in equilibrium at all stages of compression, so that the product of the pressure term and the volume term is a constant. where C = degree of volume reduction of a powder compact at pressure P. constants (a and b) =evaluated from a plot of P/C versus P. a= total volume reduction for the powder bed [carr’s index] b= constant that is inversely related to the yield strength of the particles. The data from this study were modeled via the Kawakita equation in an attempt to evaluate the relationship between the volume reduction and applied pressure for each studied DC binder.
CONCLUSION Compression & Consolidation are important in tableting of materials. The importance of each will largely depend on the type of compact required whether soft or hard and on the brittle properties of the materials . Various mathematical equations have been used to describe the compaction process.
CONCLUSION CONT.. The particular value of heckel plots arises from their ability to identify the predominant form of deformation in a given sample. Kawakita equation is modified form of heckel’s equation.
REFERENCES The Theory and Practice of Industrial pharmacy Leon Lachman, Herbert E. Lieberman, Joseph L. Kanic Special Indian Edition 2009 Page no.71-83. Aulton’s Pharmaceutics The design and Manufacture of Medicines Michael E. Aulton Third Edition Page no.478,443,468-473,355-358. www.google.com www.wikipedia.com